# Purification for Carbon Nanotubes Synthesized by Flame Fragments Deposition via Hydrogen Peroxide and Acetone

Asmaa Hammadi, Ahmed Jasim, Firas Abdulrazzak, Abdulkareem

Al-Sammarraie, Yacine Cherifi, Rabah Boukherroub, Falah Hussein

► To cite this version:

Asmaa Hammadi, Ahmed Jasim, Firas Abdulrazzak, Abdulkareem Al-Sammarraie, Yacine Cherifi, et al.. Purification for Carbon Nanotubes Synthesized by Flame Fragments Deposition via Hydrogen Peroxide and Acetone. Materials, 2020, 13 (10), pp.2342. 10.3390/ma13102342 . hal-03090032

HAL Id: hal-03090032

https://hal.science/hal-03090032

Submitted on 11 Jul 2022

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
Communication

# Purification for Carbon Nanotubes Synthesized by Flame Fragments Deposition via Hydrogen Peroxide and Acetone

Asmaa H. Hammadi¹, Ahmed M. Jasim² ID, Firas H. Abdulrazzak³,

Abdulkareem M. A. Al-Sammarraie⁴, Yacine Cherifi⁵, Rabah Boukherroub⁵ ID and

Falah H. Hussein¹,⁶,* ID

¹ College of Pharmacy, University of Babylon, Hilla 51002, Iraq; phar.asmaa.hashim@uobabylon.edu.iq

² Department of Biomedical, Biological and Chemical Engineering, University of Missouri, Columbia, MO 65211, USA; amjtg6@mail.missouri.edu

³ Chemistry Department, College of Education for Pure Sciences, Diyala University, Baqubah 32001, Iraq; firas.habeeb@puresci.uodiyala.edu.iq

⁴ Department of Chemistry, College of Science, University of Baghdad, Baghdad 10070, Iraq; karim.alsamuraee@uobaghdad.edu.iq

⁵ Univ. Lille, CNRS, Centrale Lille, ISEN, Univ. Valenciennes, UMR 8520-IEMN, F-59000 Lille, France; yacine.dz15@gmail.com (Y.C.); rabah.boukherroub@iemn.univ-lille1.fr (R.B.)

⁶ Pharmacy Department, Al-Mustaqbal University College, Babylon 51002, Iraq

* Correspondence: abohasan_hilla@yahoo.com

Received: 20 April 2020; Accepted: 15 May 2020; Published: 20 May 2020

<figure><img src="image_2.png" /></figure>

check for
updates

**Abstract:** Carbon nanotubes (CNTs) are synthesized by the flame fragment deposition (FFD) technique using Iraqi liquefied petroleum gas (LPG) as a source of carbon in a hand-made reactor at a low temperature (160 °C) without using a catalyst. Purification of the multi-walled carbon nanotubes (MWCNTs) is carried out using a two-step process consisting of sonication in 30 wt.% hydrogen peroxide (H₂O₂) solution at room temperature to remove amorphous impurities adhering to the walls of the CNTs and carbon nanoparticles (CNPs), followed by sonication in an acetone bath to remove the polyaromatic hydrocarbons (PAH) formed during the LPG gas burning. Comprehensive characterizations such as X-ray diffraction (XRD), atomic force microscopy (AFM), thermo-gravimetric analysis (TGA), and transmission electron microscopy (TEM) were conducted to verify the efficiency of the purification process. The results clearly demonstrated that this process is promising for the purification of the synthesized CNTs.

**Keywords:** flame fragments deposition; hydrogen peroxide; liquefied petroleum gas; CNTs purification

## 1. Introduction

Since their discovery in 1990 [1], carbon nanotubes (CNTs) have attracted remarkable interest because of their unique physical [2], chemical [3], and mechanical properties [4,5]. They have been used in various applications such as catalysis [6], biotechnology and biomedicine [7,8], probing of field emission stability [9], and even as a template to make some metal oxide nanostructures [10]. Upon the synthesis processes, the fresh surface has a lot of impurities such as amorphous carbon (non-crystallized), catalyst metals, and so on. Since most of the CNTs modern application depends on their purity, several procedures have been developed for their purification. The purification techniques are classified to three main methods, namely physical, chemical, and the combination of chemical and physical methods [11]. All the purification methods deal with one target, which is the removal of amorphous carbon, carbon nanoparticles, and the residual catalyst that was used in
CNTs synthesis [12–14]. Each technique presents one or more disadvantages such as non-selectivity, damage of nanotubes, formation of toxic wastes, and time consumption. The physical methods such as ultrasonication, filtration, and centrifugation are considered as mild and less effective methods, however, they do not destroy the pristine structure [15–17]. In chemical purification, there are two routes including dry and wet conditions. The dry refers to oxidation under air [18], oxygen, and other gases [19], while the wet conditions refer to using of strong liquid oxidants. Martinez et al. [20] purified SWNTs by a combination of air treatment/microwave, leading to a high metal removal within a short time as compared with acid reflux treatments. Gomez et al. [21] used a method for purification that consists of two steps. The first one is treatment in a microwave and the second step consists of a gas-phase chlorination. Piranha mixtures whether the acidic solution (H₂SO₄/H₂O₂) or the alkaline solution (NH₄OH/H₂O₂) [22] are used in the wet oxidation. The CNTs purification in nitric acid was also reported [23,24]. The nitric acid purification results in an effective purification as they able to unzip the tube wall removing the amorphous carbon as well as the metal catalyst. However, it is destructive and could damage the pristine structure of the CNTs backbone. Other people have found potassium permanganate (KMnO₄) to be an effective oxidant [25]. Colomer et al. [26] have reported an effective oxidation using KMnO₄ by applying a low temperature of 80 °C and found, through transmission electron microscopy (TEM) imaging, all the amorphous aggregates were removed. Unfortunately, when KMnO₄ is used, further steps are required such as a long washing time to remove the formed MnO₂ [27].

On the other hand, hydrogen peroxide H₂O₂ was found to be a promising oxidant that is capable to attack the carbon surface without destroying the pristine structure of the CNTs, requiring less washing times, and not to mention that it produces water as a by-product [28]. Rasel et al. [29] investigated other mixtures of chemical agents for purifying MWNTs such as a mixture of hydrogen peroxide with KOH or HCl. HCl/H₂O₂ showed 100% purification as compared to HCl and KOH/H₂O₂ with purification yields of 93.46% and 3.92%, respectively. Nevertheless, the use of H₂O₂ solely at a low concentration lacks the capability to remove metal traces embedded in the CNTs structure wall. Suzuki et al. [30] have reported an efficient purification method of arc-plasma-single wall carbon nanotubes (SWCNT) by reflux in a H₂O₂ solution in the presence of iron particles as a catalyst. Their results showed a 90% purification by removing all the amorphous carbon material. They attributed that to the active oxygen that was created by the reaction between iron and H₂O₂.

Herein, we have synthesized carbon nanotubes with no need for a catalyst. Thus, H₂O₂ oxidation could perfectly fit. It was followed by a purification in acetone to ensure dissolving any left-over organic residues originated from the used LPG gas. This process was compared with only H₂O₂. We observed the influence of both oxidation techniques on thermal stability by using thermogravimetric analysis (TGA). The oxidation by H₂O₂ followed by acetone washing method showed a higher thermal stability of the CNTs than those purified only through oxidation with H₂O₂. The changes in the morphology were monitored using transmission electron microscopy (TEM) and atomic force microscopy (AFM). The structure was further examined by powder X-ray diffraction (XRD). We envision that the sequential purification with hydrogen peroxide and acetone could provide an effective, environmentally friendly, and less expensive technique.

## 2. Materials and Methods

### 2.1. Materials

Iraqi liquefied petroleum gas (LPG) was purchased from the local market in Babylon Governorate. The materials used in this experiment was methanol (99.85%) from Hyman, England, acetone (99%) from S.D. Fine-chem. Ltd., City, India and hydrogen peroxide (30% H₂O₂) from Barcelona, Scharlab Spain. The N₂ (99.999%) gas was purchased from Emirates industrial gases, Dubai, United Arab Emirates. The standard MWNTs, used for comparison with synthesized CNTs in this study with a
purity of 95% and mode diameter of 5.5 nm were purchased from Aldrich. All materials were used
without further purification.

## 2.2. Carbon Nanotubes Synthesis

The Flame Fragments Deposition (FFD) process was performed using a homemade chamber instrument constructed for the synthesis of carbon nanotubes (CNTs) from LPG as the carbon source [31]. The homemade FFD instrument consists of two stainless steel boxes. The internal box (41 × 38 × 25 cm³), LPG, oxygen, and nitrogen gases were connected to the system through three stainless inlet tubes with a diameter of 1.5 cm. The flow rate of gases was controlled by outside gauges. The instrument consists of a gas gate for the excess gases. On the top of the box, there are nine positions fitted to hold the crucibles used as sample collectors. These collectors are in touch with the cold upper lid. The outer box was designed with dimensions of 50 × 47 × 38 cm³. The outer box has an airtight cover. The instrument has a front lens with dimensions of 14 × 13 cm², used to monitor the intensity of the flame. The schematic diagram of the homemade flame fragments deposition instrument is shown in Figure 1.

<figure><img src="image_3.png" /><figcaption>**Figure 1.** The homemade flame fragments deposition (FFD) instrument.</figcaption></figure>

## 2.3. Purification Processes

Two routes were used for the purification of the synthesized CNTs. The first is an oxidation with H₂O₂, while the second one consists of an oxidation with H₂O₂ followed by acetone treatment using a separation funnel. 100 mg of as-prepared CNTs were dispersed with an ultrasonic water bath in 50 mL of H₂O₂ for one hour. The mixture was left in a refrigerator at 4 °C for 24 h, after that, the solution allowed to reach room temperature then heated gradually to 50 °C until all hydrogen peroxide was completely destroyed. Finally, the sample was washed with deionized water and dried at 80 °C for 4 h. The second route comprises the same steps with an additional washing step with acetone of the dried sample. The treatment with acetone includes dispersion of CNTs in 15 mL of acetone and sonication for 15 min. The suspension was then centrifuged for 15 min. The separated CNTs were then calcined at 275 °C for 2 h.

## 2.4. Characterizations

The X-ray diffraction (XRD) patterns were performed on a (RU-200B) (Rigaku, Tokyo, Japan) X-ray diffractometer using Cu Kα radiation (wavelength = 0.15405 nm) with a Ni filter. The tube current was 100 mA with a tube voltage of 40 kV. The 2θ angular region between 10 and 80° was
explored at a scan rate of 5 °/min. For all the XRD analysis, the resolution in the 2θ scans was kept at 0.02°. Initial transmission electron microscopy (TEM) measurements to confirm morphology were performed using JEOL JEM-1400 (Jeol Inc., Peabody, MA, USA) equipped with Lanthanum-hexaboride (LaB₆) filament and operated at an acceleration voltage 120 kV and data were collected on the Gatan Ultrascan 1000 CCD camera (Thermo Fisher Scientific, Hillsboro, OR, USA). Subsequent measurements were performed using FEI Tecnai F30 Twin microscope (Thermo Fisher Scientific, Hillsboro, OR, USA) equipped with analytical spectrometers (Bruker Quantax 400 Silicon Drift Detector or Quantum 963 Gatan Image filter (GIF)) to get high magnified TEM images. Atomic Force Microscopy (AFM) was performed by placing a well-dispersed droplet of CNTs ink using (SPM-A3000, Angstrom Advanced Inc., Stoughton, MA, USA, Atomic force microscopy (AFM)-Contact mode).

### 3. Results and Discussion

Atomic force microscopy (AFM) is a highly powerful tool [32] with a high resolution less than a few nanometers. Therefore, using such tool provides us a sense on how the material topography is distributed. In Figure 2, the AFM image shows the samples in 2-D and 3-D before and after treatment in hydrogen peroxide and acetone. Figure 2a,b depicts the material as bundles or quaffs of carbon filaments consisting of minimal fraction CNTs. Many aggregations are present resulting from remaining particles on the surface. The existence of heavy oil materials as part of LPG, which form agglomerates can be considered as the reason behind such morphology. Even though there are some CNTs, their hydrophobic surface nature leads to their agglomeration through Van der Waals forces [33]. After treating the above product with hydrogen peroxide and acetone in a sequential process, the AFM shows a tubular structure with a pattern of bundles as in Figure 2c,d. It is important to mention that H₂O₂ solely failed to decompose the oil materials. Nevertheless, the synthesized CNTs after sequential treatment with H₂O₂ followed by acetone has shown a descent evidence of having CNTs structure with a length of 0.8–2.1 µm with a tubular structure.

<figure><img src="image_4.png" /><figcaption>**Figure 2.** Atomic force microscopy (AFM) images of produced MWNTs: (a,b) 2-D and 3-D sections before any treatment, (c,d) 2-D and 3-D sections after treatment by hydrogen peroxide and acetone.</figcaption></figure>
Figure 3a displays a low-resolution transmission electron microscopy (TEM) image of synthesized CNTs before any purification. It can be seen that the unconverted carbon is wrapping the CNTs bundles. However, these impurities were removed after the CNTs exposure to H₂O₂ then acetone. Figure 3b depicts the TEM image of the CNTs after treatment with H₂O₂ and acetone. Hydrogen peroxide removes the impurities without damaging the CNTs or forming any byproduct such salts, which may adsorb on the inner or outer part of the tubular structure. The influence of H₂O₂ is not only limited to purification but can also serve to functionalize the outer surface of CNTs. The functionalization process of the CNTs surface produces C-O, C=O, and C-OH groups, which reduces Van der Walls forces between CNTs bundles, allowing to visualize the CNTs as single filaments.

<figure><img src="image_5.png" /><figcaption>**Figure 3.** Transmission electron microscopy (TEM) images: (a) before treatment, (b) after treatment with H₂O₂ and acetone, and (c) high-resolution images with graphite inner plans (lattices masked by Gatan Software 3.0).</figcaption></figure>

For further investigation, high-resolution imaging was conducted to check the surface structure. Figure 3c depicts a TEM image at an acceleration voltage of 200 kV showing the graphite lattice interplanar spacing of 0.35 nm (as in the inset). The high-resolution image is highly crucial since it provides information on the synthesized material whether it is CNTs or CNFs. We observed a high crystallinity on the outer wall with a thin film of amorphous film. This indicates that the synthesized material is neither fully crystalline nor amorphous. To resolve such ambiguity, X-ray diffraction (XRD) was recorded to gain more insights. Figure 4 displays the XRD pattern of MWNTs obtained from Aldrich for comparison purpose as a benchmark. It exhibits two characteristic peaks at 2θ = 26.32° and 43.46° assigned to the C (100) and C (002) planes of the carbon nanotubes, respectively [34]. The synthesized CNTs show similar peaks at 2θ = 26.56° and 44.16° after treatment with H₂O₂/acetone. However, impurities appear in the sample before treatment with H₂O₂/acetone with four distinguished
peaks at 2θ = 14.78°, 29.47°, 31.86°, and 49.38°. The peaks at 2θ = 14.78° and 29.47° can be assigned to remaining and unconverted carbon, while the second two peaks refer to aluminum used as support for precipitation [35]. Regarding the surface graphitizing degree, all samples show peaks, indicating that crystalline structure planes are present.

<figure><img src="image_6.png" /><figcaption>**Figure 4.** X-ray diffraction (XRD) patterns of multi-walled carbon nanotubes (MWCNTs) from Aldrich and the synthesized carbon nanotubes (CNTs) after purification with H₂O₂/acetone.</figcaption></figure>

Thermo-gravimetric analysis (TGA) is commonly used to assess the purity and quality of the synthesized CNTs, because the support and support/catalyst influence directly CNTs purity and type. The temperature at which a carbon material is oxidized is an indication of its stability. Typically, it is used to obtain a semi-quantitative estimation of the fraction of CNT in a sample, but it is not a precise quantitative technique. Figure 5a shows the TGA thermogram recorded under nitrogen gas for MWNTs from Aldrich, which reveals that the mass loss occurs in two steps. At 200 °C < T < 400 °C, a first mass loss of about 1.43% that can be attributed to the surface adsorbed water which is supported by the endothermic peak, as seen in derivative temperature curve. Above 400 °C, about 8.97% loss takes place related to some left-over amorphous material attached to graphic structure of MWNTs.

Figure 5b represents the thermal analysis of the prepared CNTs sample after treatment with only H₂O₂. It shows two steps: at T < 400 °C, there is a mass loss of about 4.3% that can be attributed to the evaporation of water and heavy organic material introduced through the deposition process [33]. In the 400-800 °C temperature range, a mass loss of 13.4% was observed due to the decomposition of more organic compounds on the CNTs such as amorphous carbon or traces of PAH residues.

Figure 5c exhibits the TGA thermogram of CNTs after treatment with H₂O₂/acetone, revealing 1.8% mass loss up to 400 °C, which is slightly lower than the mass loss recorded for CNTs after treatment with H₂O₂. Most of the mass loss is initiated at 390 °C and equals to 14.03%. In total, the sample lost 15.47 wt.% from heating to 800 °C and the ratio of CNTs was 84.53%. The difference of the thermal behavior of CNTs treated with H₂O₂ and H₂O₂/acetone in the 30-400 °C temperature range may be due to successful removal of oils materials by acetone.
<figure><img src="image_7.png" /><figcaption>**Figure 5.** Thermo-gravimetric analysis (TGA) thermograms of: (a) MWNTs (Aldrich), (b) CNTs treated with hydrogen peroxide, and (c) treated with hydrogen peroxide then acetone.</figcaption></figure>

**4. Conclusions**

In this work, we have demonstrated that flame fragments deposition (FFD) method using Iraqi LPG as a source of carbon in a hand-made reactor at low temperature (160 °C) without using a catalyst can be successfully applied for the synthesis of carbon nanotubes. The obtained crude CNTs are covered with amorphous carbon and polycyclic aromatic hydrocarbons. Two chemical protocols have been tested to purify the crude CNTs, consisting of hydrogen peroxide (H₂O₂) or H₂O₂/acetone treatment. While H₂O₂ treatment allows one to remove the amorphous carbon layer, H₂O₂/acetone turned out to be a good method for the purification of synthesized CNTs, exhibiting the higher thermal stability when eliminating the interference materials. TEM reflected carbon quantum dots decorated CNTs, which extends their properties for new advanced applications.
**Author Contributions:** Conceptualization, F.H.H. and A.H.H.; methodology, F.H.A. and A.M.A.A.-S.; draft preparation, A.H.H., and A.M.J.; TEM characterization, A.M.J.; writing—review, A.H.H., A.M.J., F.H.A., A.M.A.A.-S., Y.C., R.B. and F.H.H. All authors have read and agreed to the published version of the manuscript.

**Funding:** No external funding was provided.

**Conflicts of Interest:** The authors declare no conflict of interest.

## References

1. Iijima, S.; Ichihashi, T.J.N. Single-shell carbon nanotubes of 1-nm diameter. *Nature* **1993**, *363*, 603. [CrossRef]

2. Hines, R.; Hajilouezhad, T.; Love-Baker, C.; Koerner, G.; Maschmann, M.R. Growth and Mechanics of Heterogeneous, 3D Carbon Nanotube Forest Microstructures Formed by Sequential Selective-Area Synthesis. *ACS Appl. Mater. Interfaces* **2020**, *12*, 17893–17900. [CrossRef] [PubMed]

3. Jasim, A.M.; Hoff, S.E.; Xing, Y.J.E.A. Enhancing methanol electrooxidation activity using double oxide catalyst support of tin oxide clusters on doped titanium dioxides. *Electrochim. Acta* **2018**, *261*, 221–226. [CrossRef]

4. Hajilouezhad, T.; Ajiboye, D.M.; Maschmann, M.R. Evaluating the Forces Generated During Carbon Nanotube Forest Growth and Self-Assembly. *Materialia* **2019**, *7*, 100371. [CrossRef]

5. Ibrahim, K.S. Carbon nanotubes—properties and applications: A review. *Carbon Lett.* **2013**, *14*, 131–144. [CrossRef]

6. Jasim, A.M. *Enhancing Methanol Electro-Oxidation by Double Oxide Incorporation with Platinum on Carbon Nanotubes*; University of Missouri: Columbia, MO, USA, 2016.

7. Bekyarova, E.; Ni, Y.; Malarkey, E.B.; Montana, V.; McWilliams, J.L.; Haddon, R.C.; Parpura, V. Applications of carbon nanotubes in biotechnology and biomedicine. *J. Biomed. Nanotechnol.* **2005**, *1*, 3–17. [CrossRef]

8. Alwindawi, H.; Ismail, S.; Nafaee, Z.; Salman, H.; Balakit, A.; Hussein, F. Comparison between Biological Activities of Commercial and Synthesized Carbon Nanotubes by Flame Fragments Deposition Technique. *Baghdad Sci. J.* **2019**, *16*, 878–885.

9. Giubileo, F.; Di Bartolomeo, A.; Scarfato, A.; Iemmo, L.; Bobba, F.; Passacantando, M.; Santucci, S.; Cucolo, A. Local probing of the field emission stability of vertically aligned multi-walled carbon nanotubes. *Carbon* **2009**, *47*, 1074–1080. [CrossRef]

10. Jasim, A.M.; He, X.; White, T.A.; Xing, Y. Nano-layer deposition of metal oxides via a condensed water film. *Commun. Mater.* **2020**, *1*, 9. [CrossRef]

11. Hou, P.-X.; Liu, C.; Cheng, H.-M. Purification of carbon nanotubes. *Carbon* **2008**, *46*, 2003–2025. [CrossRef]

12. Ismail, A.; Goh, P.S.; Tee, J.C.; Sanip, S.M.; Aziz, M. A review of purification techniques for carbon nanotubes. *Nano* **2008**, *3*, 127–143. [CrossRef]

13. MacKenzie, K.; Dunens, O.; Harris, A.T. A review of carbon nanotube purification by microwave assisted acid digestion. *Sep. Purif. Technol.* **2009**, *66*, 209–222. [CrossRef]

14. Wang, F.; Matsuda, K.; Rahman, A.M.; Peng, X.; Kimura, T.; Komatsu, N. Simultaneous discrimination of handedness and diameter of single-walled carbon nanotubes (SWNTs) with chiral diporphyrin nanotweezers leading to enrichment of a single enantiomer of (6, 5)-SWNTs. *J. Am. Chem. Soc.* **2010**, *132*, 10876–10881. [CrossRef] [PubMed]

15. Salernitano, E.; Giorgi, L.; Makris, T.D.; Giorgi, R.; Lisi, N.; Contini, V.; Falconieri, M. Purification of MWCNTs grown on a nanosized unsupported Fe-based powder catalyst. *Diam. Relat. Mater.* **2007**, *16*, 1565–1570. [CrossRef]

16. Tagmatarchis, N.; Zattoni, A.; Reschiglian, P.; Prato, M. Separation and purification of functionalised water-soluble multi-walled carbon nanotubes by flow field-flow fractionation. *Carbon* **2005**, *43*, 1984–1989. [CrossRef]

17. Yang, C.; Hu, X.; Wang, D.; Dai, C.; Zhang, L.; Jin, H.; Agathopoulos, S. Ultrasonically treated multi-walled carbon nanotubes (MWCNTs) as PtRu catalyst supports for methanol electrooxidation. *J. Power Sources* **2006**, *160*, 187–193. [CrossRef]

18. Li, C.; Wang, D.; Liang, T.; Wang, X.; Wu, J.; Hu, X.; Liang, J. Oxidation of multiwalled carbon nanotubes by air: Benefits for electric double layer capacitors. *Powder Technol.* **2004**, *142*, 175–179. [CrossRef]

19. Smith, M.R., Jr.; Hedges, S.W.; LaCount, R.; Kern, D.; Shah, N.; Huffman, G.P.; Bockrath, B. Selective oxidation of single-walled carbon nanotubes using carbon dioxide. *Carbon* **2003**, *41*, 1221–1230. [CrossRef]
20. Martinez, M.; Callejas, M.; Benito, A.M.; Maser, W.K.; Cochet, M.; Andres, J.; Schreiber, J.; Chauvet, O.; Fierro, J. Microwave single walled carbon nanotubes purification. *Chem. Commun.* **2002**, *1000–1001*. [CrossRef]

21. Gomez, V.; Irusta, S.; Lawal, O.B.; Adams, W.; Hauge, R.H.; Dunnill, C.W.; Barron, A.R. Enhanced purification of carbon nanotubes by microwave and chlorine cleaning procedures. *Rsc Adv.* **2016**, *6*, 11895–11902. [CrossRef]

22. Chia, J.S.Y.; Tan, M.T.; Chin, J.K.; Khiew, P.S.; Lee, H. A parametric study on the synthesis of graphene using Piranha-like thermal exfoliation. *IPCBEE* **2012**, *48*, 143.

23. Abdulrazzak, F.H.; Esmail, S.K.; Dawod, H.A.; Abbas, A.M.; Almaliki, M.K. X-ray Analysis for Purification Process of Synthesized Multi-Walled Carbon Nanotubes by Chemical Vapor Deposition. *Int. J. Theor. Appl. Sci.* **2016**, *8*, 37.

24. Ko, F.-H.; Lee, C.-Y.; Ko, C.-J.; Chu, T.-C. Purification of multi-walled carbon nanotubes through microwave heating of nitric acid in a closed vessel. *Carbon* **2005**, *43*, 727–733. [CrossRef]

25. Azodpour, J.; Baniadam, M. Microwave assisted purification of multi-walled carbon nanotubes by potassium permanganate; effect of acid to oxidant molar ratio and treatment time. *Diam. Relat. Mater.* **2019**, *98*, 107485. [CrossRef]

26. Colomer, J.-F.; Piedigrosso, P.; Fonseca, A.; Nagy, J.B. Different purification methods of carbon nanotubes produced by catalytic synthesis. *Synth. Met.* **1999**, *103*, 2482–2483. [CrossRef]

27. Hernadi, K.; Siska, A.; Thien-Nga, L.; Forro, L.; Kiricsi, I. Reactivity of different kinds of carbon during oxidative purification of catalytically prepared carbon nanotubes. *Solid State Ion.* **2001**, *141*, 203–209. [CrossRef]

28. Feng, Y.; Zhang, H.; Hou, Y.; McNicholas, T.P.; Yuan, D.; Yang, S.; Ding, L.; Feng, W.; Liu, J. Room temperature purification of few-walled carbon nanotubes with high yield. *ACS Nano* **2008**, *2*, 1634–1638. [CrossRef]

29. Das, R.; Ali, M.E.; Hamid, S.B.A.; Annuar, M.; Ramakrishna, S. Common wet chemical agents for purifying multiwalled carbon nanotubes. *J. Nanomater.* **2014**, *2014*, 237. [CrossRef]

30. Suzuki, T.; Suhama, K.; Zhao, X.; Inoue, S.; Nishikawa, N.; Ando, Y. Purification of single-wall carbon nanotubes produced by arc plasma jet method. *Diam. Relat. Mater.* **2007**, *16*, 1116–1120. [CrossRef]

31. Hammadi, A.H.; Abdulrazzak, F.H.; Atiyah, A.J.; Hussein, F.H. Synthesis of Carbon Nano tubes by Flame Fragments Deposition of Liquefied Petroleum Gas. *Org. Med. Chem. IJ* **2017**, *29*, 2804–2808. [CrossRef]

32. Toader, M.; Fiedler, H.; Hermann, S.; Schulz, S.E.; Gessner, T.; Hietschold, M. Conductive AFM for CNT characterization. *Nanoscale Res. Lett.* **2013**, *8*, 1–6. [CrossRef] [PubMed]

33. Dikio, E.D.; Shooto, N.D.; Thema, F.T.; Farah, A.M. Raman and TGA study of carbon nanotubes synthesized over Mo/Fe catalyst on aluminium oxide, calcium carbonate and magnesium oxide support. *Chem. Sci. Trans.* **2013**, *2*, 1160–1173.

34. Ebbesen, T.; Ajayan, P.; Hiura, H.; Tanigaki, K. Purification of nanotubes. *Nature* **1994**, *367*, 519. [CrossRef]

35. Rebhi, A.; Makhlouf, T.; Njah, N. X-Ray diffraction analysis of 99.1% recycled aluminium subjected to equal channel angular extrusion. *Phys. Procedia* **2009**, *2*, 1263–1270. [CrossRef]

<figure><img src="image_8.png" /></figure>

© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).